Research Article  Open Access
Anju K. Augustine, S. Mathew, P. Radhakrishnan, V. P. N. Nampoori, M. Kailasnath, "Size Dependent Optical Nonlinearity and Optical Limiting Properties of Water Soluble CdSe Quantum Dots", Journal of Nanoscience, vol. 2014, Article ID 623742, 7 pages, 2014. https://doi.org/10.1155/2014/623742
Size Dependent Optical Nonlinearity and Optical Limiting Properties of Water Soluble CdSe Quantum Dots
Abstract
We present thirdorder optical nonlinear absorption in CdSe quantum dots (QDs) with particle sizes in the range of 4.16–5.25 nm which has been evaluated by the scan technique. At an excitation irradiance of 0.54 GW/cm^{2} the CdSe QDs exhibit reverse saturation indicating a clear nonlinear behavior. Nonlinearity increases with particle size in CdSe QDs within the range of our investigations which in turn depends on the optical band gap. The optical limiting threshold of the QDs varies from 0.35 GW/cm^{2} to 0.57 GW/cm^{2} which makes CdSe QDs a promising candidate for reversesaturable absorption based devices at high laser intensities such as optical limiters.
1. Introduction
Before the advent of lasers, transparent optical materials were assumed to be essentially passive unaffected by the light travelling through them. The high powers of laser beams made it possible to observe that the effect of light on a medium can indeed change its properties such as refractive index or absorption. These are optical nonlinear phenomena. When this happens, the light itself gets affected by this change in a nonlinear way; for example, the nonlinear response of the material can convert the laser light into new colours, both harmonics of the optical frequency and sum and difference frequencies. With the development of optical communication networks, various nonlinear optical (NLO) devices such as optical switches, optical limiters, optical detectors, and optical sensors have attracted considerable attention because of their widespread usage for scientific and industrial purposes. Among all the NLO properties, optical limiting is one of the most promising practical applications, as it can protect the human eye and photosensitive components from damage caused by intense optical radiation [1, 2]. Optical limiting results from irradiancedependent NLO responses of materials in which the incoming intense light alters the refractive and absorptive properties, resulting in a greatly reduced transmitted intensity. It is important to select suitable materials as optical limiting media by determining the magnitude of their nonlinearity. Organic materials characterized by large NLO responses are of major interest owing to their large NLO susceptibilities, fast response time, architectural flexibility, low cost, and ease of fabrication [3, 4].
In recent years, interest in the synthesis, characterization, and application of colloidal quantum dot (QD) semiconductor materials has grown markedly. QDs of cadmium selenide (CdSe) are by far the most studied system among all the semiconducting nanocrystals. The bulk CdSe has a direct band gap of 1.74 eV at 300 K and a typical Bohr exciton diameter of around 5.6 nm [5]. Consequently, CdSe QDs show sizable quantum confinement effects with remarkably different optical properties. The size dependent, unusual optical and electronic properties of these QDs have been studied in detail using a wide variety of experimental and theoretical techniques. The linear optical properties of CdSe QDs depend strongly on particle size; for example, the blue shift of excitonic absorption and emission peaks with decreasing particle size is a wellknown observation. The unusual properties of the QDs, in the quantumconfined regime, have led to numerous technological applications.
In the past decade, there has been increasing interest in the luminescent and nonlinear optical properties of these nanometersized QDs. Large optical nonlinearities in CdSe QDs have been reported using different techniques. These techniques include degenerate fourwave mixing and scan techniques with nanosecond and picosecond laser pulses. scan, especially, is an effective technique to investigate nonlinear absorption and nonlinear refraction. An ideal optical limiter, by definition, is a device that exhibits a linear transmittance below a threshold and clamps the output to a constant above it, thus providing safety to sensors and the eyes. A wide range of materials contributing to the optical limiting and nonlinear absorption has been investigated. It is well known that optical limiting devices rely on one or more of the nonlinear optical mechanisms such as excited state absorption, free carrier absorption, twophoton absorption (TPA), thermal defocusing/scattering, photorefraction, nonlinear refraction, and induced scattering with enhancement in limiting performance by coupling two or more of such mechanisms [6–8].
In this paper, we present the study of the effect of size on the nonlinear optical properties of CdSe QDs and estimate the nonlinear absorption coefficient of CdSe QDs at different particle size at 532 nm. These CdSe QDs exhibit reverse saturable absorption (RSA), in which the excited state absorption cross section is higher than the ground state absorption cross section. The origin of the thirdorder nonlinearity predicted from scan studies is attributed to resonant twophoton absorption (TPA). We also report the limiting threshold as a function of the particle size of CdSe QDs.
2. Experimental
In the present work, CdSe NPs were prepared by a modified aqueous method using reflux [9, 10]. The precursors used are CdCl_{2} : H_{2}O and Na_{2}SeO_{3}. The capping agent used was mercaptosuccinic acid (MSA). The molar ratio of the precursors and MSA is 4 : 1 : 12, respectively. The buffer solution [11] with pH~7 is prepared with sodium borate and citric acid in water. The precursors were added to the buffer with constant stirring. The pH of the corresponding colourless solution is adjusted by adding 1 M NaOH. It was placed in a threenecked flask followed by reflux at 100°C in openair conditions. Reflux process gives the required thermal energy to the reaction. The colour of the solution turned to bright yellow after a few minutes of reflux. The temperature of the reaction system was maintained at 100°C. During the reflux, the colour of solution gradually changed and NPs started to form and aliquots were taken out of the flask at different times for the optical measurements to monitor the growth of the QDs. The particles tend to form agglomerates due to the strong interaction of the carboxylic groups [11] leading to a possible overestimation of the mean size distribution.
Absorption spectra of the prepared CdSe QDs were recorded using UVVisible Spectrophotometer (Jasco V570 UV/VIS/IR). Fluorescence spectra of QDs were obtained on a Cary Eclipse Fluorescence Spectrophotometer (Varian). The excitation wavelength was kept at 390 nm, and the emission spectra were recorded. All absorption and fluorescence spectra were measured without any postpreparative size separation. The structural properties of the samples were investigated by Xray diffraction (XRD) on a Bruker AXS D8 Advance Xray diffractometer with Nifiltered Cu Kα (1.5406 Å) source. The electron micrograph images of CdSe QDs in colloidal form were taken using transmission electron microscope (Philips Tecnai G2 at 120 kV). The FTIR spectra of the samples were recorded using Thermo NICOLET 380 FTIR Spectrometer by means of KBr pellet procedure. Nonlinear absorption coefficient and optical limiting threshold of the samples were calculated using open aperture scan technique employing an NdYAG laser (532 nm, 7 ns, 10 Hz). The experimental setup is shown in Figure 1.
3. Results and Discussion
For detailed study, we used samples taken after reflux times of 10 minutes, 1 hour, and 3 hours and they are denoted by C_{1}, C_{2}, and C_{3}, respectively. The variation in absorption peak and the corresponding optical energy band gap (inset) of samples (C_{1}, C_{2}, and C_{3}) are shown in Figures 2(a), 2(b), and 2(c).
(a)
(b)
(c)
Energy band gap of the QDs shows a variation from 2.51 eV to 2.34 eV as the particle size increased during the reflux time from 10 minutes to 3 hours. It is observed that as particle size increases, absorption peak shifts to higher wavelength side and the band gap is enhanced with decrease in particle size. The emission spectra of the C_{1}, C_{2}, and C_{3} samples are also shown in Figure 3.
(a)
(b)
(c)
The particle size is calculated with effective mass approximation [12]. For CdSe, eV, , , : where is the particle diameter. The calculated particle size of these QDs is presented in Table 1. A typical XRD spectrum of CdSe QDs is shown in Figure 4 and the average particle size can be measured using Scherrer equation , where is the full width at half maximum of the peak.

The calculated average particle size is about 4 nm for the powdered sample. The peak observed at (hkl) values of 27° (101), 35° (102), 41° (110), 50° (201), and 55° (202) planes shows the existence of CdSe hexagonal phase (JCPDS file no. 010712554).
Figure 5(a) shows histogram and TEM image of C_{3} sample with average particle size of 4.09 nm. It shows that the particles formed are in spherical shape and average particle size is calculated to be 4.09 nm. Figure 5(b) represents HRTEM image of C_{3} sample which suggests that the prepared CdSe QDs have good crystallinity and this may enable them to possess highquality optical property.
(a)
(b)
FTIR spectrum of the C_{3} sample is shown in Figure 6. A broad peak at 3430 cm^{−1} is assigned to –OH stretching. The Cd–Se band stretching can be observed at ~843 cm^{−1}. The double peaks of the carboxylate vibration at 1587 cm^{−1} (in the range 1540–1650 cm^{−1}, asymmetric) and 1403 cm^{−1} (in the range 1360–1450 cm^{−1}, symmetric) in the spectra of CdSe particles show that the organics exist as carboxyl salts on the particle surface. The peak position of this doublet is similar to that observed for other mercaptocarboxylic salts.
The nonlinear optical characterization of the samples was carried out using the scan technique at 532 nm [13, 14]. The samples to be investigated were translated through the focal point of a lens of focal length of 20 cm. The beam waist radius was estimated to be 35.4 m. The Rayleigh length was calculated to be 7.4 mm. The samples were taken in a 1 mm cuvette which is much less than which is an essential prerequisite for scan experiment. The normalized transmittance for TPA in the open aperture condition is given by [15] where The parameter is the depth of the open aperture scan curve obtained from the theoretical fit and it is the measure of the intensity dependent absorption. Here, is the laser intensity in the focal plane, is the nonlinear optical absorption coefficient, and is the effective thickness with linear absorption coefficient .
is given by
The openaperture curve exhibits a normalized transmittance valley at the focal point, indicating the presence of reverse saturable absorption (RSA) in the nanocolloidal solutions. The open aperture scan plot for samples having different particle size is depicted in Figure 7. The fits of (2) to experimental data are shown as solid curves.
The data can be fitted well by assuming twophoton absorption (TPA) in the nonlinear optical absorption process. From this fit, we can confirm that the basic mechanism involved in the nonlinear absorption of nanocolloidal solutions of CdSe QDs is TPA process because the photon energy of the 532 nm laser is within the range , where eV [15]. The nonlinear absorption coefficient calculated from the above fits shows a dependence on the particle size of the QDs. The experimental data show that value increases with increasing particle size. With a small decrease in the band gap, a significant increase in the nonlinear absorption is observed. In order to explain the optical nonlinearity, we mainly consider the band gap variation of CdSe QDs samples (C_{1}, C_{2}, and C_{3}).
C_{1} and C_{2} samples have band gap very near to 2.4 (2.39 ± 0.02) and 2.5 (2.52 ± 0.02), respectively, which is more than onephoton energy corresponding to 532 nm. The data fitting shows that the nonlinear optical absorption is through twophoton absorption process in these samples. Our studies show that sample C_{3 }has large optical nonlinearity (2.47 × 10^{−10} m/W) enhancement, compared to other samples as seen in Figure 7.
Band gap corresponding to this sample is 2.33 eV to 2.33 ± 0.02 eV which is very near to the onephoton energy corresponding to 532 nm (2.33 eV). The fact that optical nonlinearity in this case is also due to the twophoton absorption reveals that twophoton excitation cross section is enhanced due to resonant onephoton absorption level. A small mismatch between band gap of sample C_{3} and one by photon energy will be compensated by phononassisted excitation. The enhancement also arises due to increased optical nonlinear interaction between the radiations and the particles. This can be explained by the fact that, with increase in particle size, there is an increase in the multiple scattering from the QDs. This increase in multiple scattering leads to large effective interaction length which in turn results in an enhancement in nonlinear absorption [14].
The open scan scheme was also used to measure . The imaginary part of thirdorder susceptibility, , is related to through the following equation: where is the linear refractive index of CdSe, is the velocity of light in vacuum, and is the angular frequency of the radiation used. The measured values of optical band gap for different particle size and nonlinear absorption coefficient at a wavelength of 532 nm for input laser power density of 0.54 GW/cm^{2} are given in Table 1.
To study the optical limiting property of the sample, the nonlinear transmission of the sample is measured as a function of input fluence. Optical power limiting is effected through the nonlinear optical processes of the sample. An important term in the optical limiting study is the optical limiting threshold. Optical limiters are essentially those systems which transmit light at low input fluence or intensities but become opaque at high inputs. The optical limiting property is mainly found to be absorptive nonlinearity, which corresponds to the imaginary part of thirdorder susceptibility [16]. From the values of fluence at focus, the fluence values at other positions could be calculated using the standard equations for Gaussian beam waist. Such plots give a better comparison of the nonlinear absorption or transmission in the sample and are generated from scan trace. Figure 8 illustrates the optical limiting response of the samples (C_{1}, C_{2}, and C_{3}).
The line in Figure 8 indicates the approximate fluence at which the normalized transmission begins to deviate from linearity. The fluence value corresponding to the onset of optical limiting (optical limiting threshold) is found to vary from 0.35 GW/cm^{2} to 0.572 GW/cm^{2} for the samples with input fluence of 0.54 GW/cm^{2}. Our work shows that the semiconductor nanomaterial which has got a onephoton resonant absorption can be employed for thirdorder optical nonlinear material in which twophoton absorption will get enhanced by the onephoton resonance energy level (Table 1). Such materials are useful as optical limiters with low threshold energy. Thus, it is clear from Figure 8 that the CdSe quantum dots with large particle size can be used for optical power limiting at high laser fluences. Thus, size of QDs has a significant effect on limiting performance.
4. Conclusion
To conclude, a simple synthetic route described in this paper permits the synthesis of highquality CdSe QDs of different particle size in aqueous solution. The MSAcapped CdSe QDs possess a tuning effect in particle size and in band gap. Linear and nonlinear optical properties were studied using optical absorption, fluorescence spectroscopy, and open aperture scan technique. The nonlinear absorption in the nanocolloidal solution can be attributed to the phenomenon of twophoton absorption. The measured values were found to enhance with decrease in optical energy gap. Our work shows that the semiconductor nanomaterial which has got a onephoton resonant absorption can be employed for thirdorder optical nonlinear material in which twophoton absorption will get enhanced by the onephoton resonance energy level.
Conflict of Interests
The authors declare that there is no conflict of interests regarding the publication of this paper.
Acknowledgments
The authors acknowledge DST for financial assistance and SAIFSTIC for XRD analysis.
References
 H. Fan, X. Wang, Q. Ren et al., “Investigation of the nonlinear absorption and optical limiting properties of two [Q]_{2}[Cu(C_{3}S_{5})_{2}] compounds,” Optics and Laser Technology, vol. 42, no. 5, pp. 732–736, 2010. View at: Publisher Site  Google Scholar
 I. Gerdova and A. Hache, “Thirdorder nonlinear spectroscopy of CdSe and CdSe/ZnS core shell quantum dots,” Optics Communications, vol. 246, no. 1–3, pp. 205–212, 2005. View at: Publisher Site  Google Scholar
 D. Maikhuri, S. P. Purohit, and K. C. Mathur, “Linear and nonlinear intraband optical properties of ZnO quantum dots embedded in SiO_{2} matrix,” AIP Advances, vol. 2, no. 1, Article ID 012160, 2012. View at: Publisher Site  Google Scholar
 N. Venkatram, R. S. S. Kumar, and D. Narayana Rao, “Nonlinear absorption and scattering properties of cadmium sulphide nanocrystals with its application as a potential optical limiter,” Journal of Applied Physics, vol. 100, no. 7, Article ID 074309, 2006. View at: Publisher Site  Google Scholar
 R. W. Meulenberg, J. R. I. Lee, A. Wolcott, J. Z. Zhang, L. J. Terminello, and T. van Buuren, “Determination of the exciton binding energy in CdSe quantum dots,” ACS Nano, vol. 3, no. 2, pp. 325–330, 2009. View at: Publisher Site  Google Scholar
 A. Patra, N. Venkatram, D. Narayana Rao, and T. P. Radhakrishnan, “Optical limiting in organic molecular nano/microcrystals: nonlinear optical effects dependent on size distribution,” Journal of Physical Chemistry C, vol. 112, no. 42, pp. 16269–16274, 2008. View at: Publisher Site  Google Scholar
 W. Sun, C. M. Lawson, G. M. Gray, C. Zhan, and D. Wang, “Degenerate fourwave mixing and Zscan measurements of stilbazolium derivatives,” Applied Physics Letters, vol. 78, no. 13, pp. 1817–1819, 2001. View at: Publisher Site  Google Scholar
 S. Mathew, A. D. Saran, B. Singh Bhardwaj et al., “Size dependent optical properties of the CdSeCdS coreshell quantum dots in the strong confinement regime,” Journal of Applied Physics, vol. 111, no. 7, Article ID 074312, 2012. View at: Publisher Site  Google Scholar
 X. Chen, J. L. Hutchison, P. J. Dobson, and G. Wakefield, “Highly luminescent monodisperse CdSe nanoparticles synthesized in aqueous solution,” Journal of Materials Science, vol. 44, no. 1, pp. 285–292, 2009. View at: Publisher Site  Google Scholar
 B. Su, D. J. Fermin, J. P. Abid, N. Eugster, and H. H. Girault, “Adsorption and photoreactivity of CdSe nanoparticles at liquidliquid interfaces,” Journal of Electroanalytical Chemistry, vol. 583, no. 2, pp. 241–247, 2005. View at: Publisher Site  Google Scholar
 A. L. Rogach, A. Kornowski, M. Gao, A. Eychmüller, and H. Weller, “Synthesis and characterization of a size series of extremely small thiolstabilized CdSe nanocrystals,” The Journal of Physical Chemistry B, vol. 103, no. 16, pp. 3065–3069, 1999. View at: Publisher Site  Google Scholar
 L. Brus, “Zerodimensional “excitons” in semiconductor clusters,” IEEE Journal of Quantum Electronics, vol. 22, no. 9, pp. 1909–1914, 1986. View at: Publisher Site  Google Scholar
 A. Thankappan, S. Thomas, and V. P. N. Nampoori, “Effect of betanin natural dye extracted from red beet root on the non linear optical properties ZnO nanoplates embedded in polymeric matrices,” Journal of Applied Physics, vol. 112, no. 12, Article ID 123104, 2012. View at: Publisher Site  Google Scholar
 I. Sebastian, S. Divya, V. P. N. Nampoori, P. Radhakrishnan, and S. Thomas, “Impact of intermediate localized states on nonlinear optical absorption of GaGeSe nanocolloidal solutions,” Applied Physics Letters, vol. 102, no. 3, Article ID 031115, 2013. View at: Publisher Site  Google Scholar
 M. SheikBahae, A. A. Said, T.H. Wei, D. J. Hagan, and E. W. Van Stryland, “Sensitive measurement of optical nonlinearities using a single beam,” IEEE Journal of Quantum Electronics, vol. 26, no. 4, pp. 760–769, 1990. View at: Publisher Site  Google Scholar
 F. M. Qureshi, S. J. Martin, X. Long et al., “Optical limiting properties of a zinc porphyrin polymer and its dimer and monomer model compounds,” Chemical Physics, vol. 231, no. 1, pp. 87–94, 1998. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2014 Anju K. Augustine et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.